LASER WELDING OF DISSIMILAR
CARBON STEEL TO STAINLESS
STEEL 316LA thesis submitted to
For the degree of
Doctor of Philosophy (PhD)
Mohammadreza Nekouie Esfahani
Dr. Sundar Marimuthu
Prof. Jeremy Coupland
Laser welding of metals and alloys is extensively used in industry due to its advantages of controlled heating, narrow weld bead, low heat affected zone (HAZ) and its ability to weld a wide range of metals and dissimilar metals. Laser welding of dissimilar metals such as carbon steels and stainless steel is still a challenging task, particularly due to the formation of brittle phases in the weld, martensitic formation in the HAZ and solidification cracking in the fusion zone. These issues can significantly deteriorate the strength of the welded joint. The aim of this work is to investigate the fundamental phenomena that occur inside the dissimilar weld zone and their effect on weld quality. In order to establish the key process variables, an initial study concentrated on the effect of different laser process parameters on dissimilar weld quality. In the second part of the work, a comprehensive study was performed to understand and subsequently control the alloying composition in laser dissimilar welding of austenitic stainless steel and low carbon steel. A dissimilar weld that is predominantly austenitic and homogeneous was obtained by controlling the melt pool dynamics through specific point energy and beam alignment. The significance of dilution and alloying elements on joint strength was established. A coupled CFD and FEM numerical model was developed to assist in understanding the melt pool dynamics and transportation processes of alloying elements. The model has been validated by a series of laser welding experiments using various levels of specific point energy. The laser welding characteristics in terms of geometric dimensions, surface morphology, alloying concentration, and dilution, were compared, and it is concluded that the specific point energy and laser beam position are the key parameters that can be controlled to obtain a weld bead with characteristics most suitable for industrial applications. In the third part of the work, a comparative study was performed to understand the significance of cooling rate, and alloying composition on the microstructure and phase structure of the dissimilar weld zone. Results show that the HAZ within the high carbon steel has significantly higher hardness than the weld area, which severely undermines the weld quality. A new heat treatment strategy was proposed based on the results of the numerical simulation, and it is shown to control the brittle phase formation in HAZ of high carbon steel. A series of experiments was performed to verify the developed thermo-metallurgical FEA model and a good qualitative agreement of the predicted martensitic phase distribution is shown to exist. Although this work is presented in the context of dissimilar laser welding of mild steel to stainless steel, the concept is applicable to any dissimilar fusion welding process.
TABLE OF CONTENTSABSTRACT ... 2 TABLE OF CONTENTS ... 3 LIST OF FIGURES ... 6 LIST OF TABLES ... 13 ACKNOWLEDGMENTS ... 14 DECLARATION ... 15 LIST OF PUBLICATIONS ... 16 LIST OF ACRONYMS ... 17
Chapter 1 Introduction to Laser Dissimilar Welding ... 18
1.1 Metal welding process ... 18
1.2 Aims and objectives of the project ... 19
1.3 Thesis structure ... 20
Chapter 2 Review of the Fundamental Theory of Laser Dissimilar Welding ... 22
2.1 Laser beam welding ... 22
2.2 Laser welding parameters ... 28
2.3 Dissimilar laser welding of metals and alloys ... 35
2.4 Melt pool dynamics in laser welding ... 41
2.5 Features of laser beam welding ... 45
2.5.1 Alloying and microstructure in laser welding ... 45
2.5.2 Weld bead geometry ... 54
2.5.3 Surface topology ... 59
2.5.4 Residual stress and service performance ... 62
2.6 Summary ... 69
Chapter 3 Materials, Methodology and Equipment ... 70
3.1 Introduction ... 70
3.2 Materials ... 70
3.3 Experimental setup ... 73
3.4 Characterization of weld quality ... 75
3.4.1 Optical microscopy and scanning electron microscopy ... 77
3.4.2 Micro-hardness and tensile testing ... 79
3.5 Design of experiments (DoE) ... 81
Chapter 4 Weld Bead Geometry and Surface Topology in Laser Dissimilar
Welding ... 86
4.1 Introduction ... 86
4.2 Previous work ... 87
4.3 Experimental procedure ... 89
4.3.1 Design of experiment ... 90
4.4 Results and discussion ... 91
4.4.1 Effect of laser power on the weld bead characteristic ... 93
4.4.2 Effect of speed on the weld bead characteristic ... 95
4.4.3 Effect of specific point energy on the weld bead characteristic ... 97
4.4.4 Effect of beam position on the weld bead characteristic ... 99
4.4.5 Statistical analysis of results ... 102
4.5 Summary ... 106
Chapter 5 Diffusion Phenomena and its Effects in Dissimilar Laser Welding ... 108
5.1 Introduction ... 108
5.2 Previous work ... 109
5.3 Experimental procedure ... 110
5.4 Results and discussion ... 114
5.4.1 Microstructure and composition in dissimilar laser welding ... 114
5.4.2 Effect of laser welding parameters on dilution and alloying elements transformation ... 117
5.4.3 Effect of laser welding parameters on microstructure ... 119
5.4.4 Effect of laser welding parameters on microhardness ... 121
5.4.5 Effect of laser welding parameters on mechanical properties ... 123
5.4.6 Effect of beam alignment on the alloying composition ... 124
5.5 Summary ... 126
Chapter 6 Numerical Simulation of Transport Phenomena in Dissimilar Laser Welding ... 128
6.1 Introduction ... 128
6.2 Previous work ... 129
6.3 Formulation and grid structure ... 130
6.3.1 Thermal analysis ... 131
6.3.2 Structural analysis ... 134
6.4 Results and discussion ... 138
6.4.1 CFD results ... 138
6.5 Summary ... 149
Chapter 7 Cooling Rate and its Effects on Dissimilar Laser Welding .... 150
7.1 Introduction ... 150
7.2 Previous work ... 151
7.3 Experimental procedure ... 153
7.4 Results and discussion ... 156
7.4.1 Microstructural evaluation ... 156
7.4.2 Effect of cooling rate and alloying composition ... 159
7.4.3 Mechanical performance of the dissimilar joint ... 163
7.5 Summary ... 165
Chapter 8 Numerical Simulation on Control of Cooling Rate in Laser Dissimilar Welding ... 166
8.1 Introduction ... 166
8.2 Previous works ... 166
8.3 Finite element modelling ... 169
8.3.1 Thermal analysis ... 169
8.3.2 Phase transformation ... 172
8.4 Results and discussion ... 173
8.5 Conclusion ... 178
Chapter 9 Conclusions and Future Work ... 179
9.1 Conclusions ... 179
9.2 Future work recommendations ... 181
References ... 183
LIST OF FIGURES
Figure 2-1 Schematic illustration of laser beam welding ... 23 Figure 2-2 Keyhole laser welding (a) Schematic of keyhole mode welding and (b) Cross-section of laser welded sample in keyhole mode  ... 24 Figure 2-3 Conduction laser welding (a) Schematic of conduction mode welding and (b) Cross-section of laser welded sample in conduction mode  ... 25 Figure 2-4 Configuration of a CO2 laser beam welding  ... 26
Figure 2-5 Comparison of heat input as a function of weld penetration depth for fibre and CO2
laser  ... 28 Figure 2-6 The relation between welding speed and penetration depth  ... 30 Figure 2-7 The effect of defocusing distance on penetration depth  ... 31 Figure 2-8 Absorption of a number of metals as a function of laser radiation wavelength of CO2 and YAG laser  ... 35
Figure 2-9 Configuration for TIG welding  ... 36 Figure 2-10 Configuration for friction stir welding  ... 37 Figure 2-11 Weld bead shape and HAZ geometry of (a) laser welded joint (power 500(W), speed 15(mm/s), argon gas pressure 1.5 (bar)) and (b) TIG welded joint (DC current 25
Ampere, non-flow rod, thoriated tungsten electrodes) ... 40 Figure 2-12 Welding of (a) Similar metals/alloys (b) Dissimilar metals/alloys  ... 41 Figure 2-13 Concave molten pool of steel formed using a CO2 laser  ... 44
Figure 2-14 Comparison of the calculated and experimentally observed laser welded fusion zone of stainless steel with outward flow as a result of negative surface tension temperature coefficient  ... 44 Figure 2-15 Comparison of the calculated and experimentally observed laser welded fusion zone of steel with inward flow as a result of positive surface tension temperature coefficient  ... 44 Figure 2-16 Variation of penetration depth, weld width and PIC as a function of peak power  ... 46 Figure 2-17 SEM microscopy and EDX result around a crack with corresponding chemical composition  ... 47
Figure 2-18 Configuration of edge-line welding  ... 47 Figure 2-19 Effect of welding speed on penetration depth and thickness (a) AZ31B (b) A5052-O  ... 48 Figure 2-20 Laser roll welding (a) Schematic of laser roll welding; (b) Side view of laser roll welding  ... 48 Figure 2-21 Formation of IMC and weld defects in Steel-Al joint  ... 49 Figure 2-22 Relationship between the weld penetration depth and the shielding gas  ... 50 Figure 2-23 Shear strength of single pass welds (600 W, 100 mm/s, f.p.p. of 0 mm) with
different shielding gases  ... 50 Figure 2-24 low carbon and stainless steel fusion zone size as a function of the laser mean power ... 52 Figure 2-25 Martensitic transformation in HAZ of carbon steel in laser dissimilar welding of carbon steel to stainless steel ... 53 Figure 2-26 Surface tension variation of stainless steel (316) with surface active elements and temperature ... 56 Figure 2-27 Variation of stainless steel (304) weld geometry with surface active elements (a) 40ppm sulphur content and (b) 140ppm sulphur content ... 56 Figure 2-28 Predicted HAZ regions in the stainless steel and the carbon steel sides according to calculated temperature distribution (°C) ... 57 Figure 2-29 Comparison of weld pool shape between simulated and experimental results with Cu on top (the colour bar on the right indicates the fraction of molten material)  ... 58 Figure 2-30 Macrographs at constant power density of 1.6MWcm-2 and specific point energy of 60J (a) Interaction time of 38ms, (b) Interaction time of 8ms  ... 58 Figure 2-31 Midpoint cross section parallel to the laser beam pass of the laser melted surface showing (a) Humping and (b) Depression  ... 59 Figure 2-32 Midpoint cross section parallel to the laser beam pass of the laser melted surface showing depression and rippling (a) Immediately after initiation of laser beam sweep (b) In steady state (c) At the end of the laser beam sweep  ... 60 Figure 2-33 Weld bead profiles and temperature contour (K) with for 600W laser power and speed: (a) 75 mm/s, (b) 100 mm/s, (c) 125 mm/s ... 61 Figure 2-34 Residual thermal distortion in dissimilar weld  (a) Experimental result, (b) Numerical result ... 64
Figure 2-35 Temperature profile and the corresponding metallographic structure ... 66
Figure 2-36 FE analysis results with and without solid-state phase transformation (S_S_P_T) longitudinal residual stresses ... 67
Figure 2-37 Microhardness profiles of the weld and HAZ (a) without PWHT and (b) with PWHT (tempered at 600 °C for 2h) ... 68
Figure 3-1 Crystallographic structures of (a) Face-centred cubic structure (fcc), and (b) Body-centred cubic structure (bcc) ... 72
Figure 3-2 Laser and workpiece configuration ... 73
Figure 3-3 1.2kW Carbon dioxide (CO2) coherent S48 laser systems ... 74
Figure 3-4 Photographic image of (a) Nozzle fibre laser welding head and (b) CO2 laser operating controller ... 75
Figure 3-5 Schematic view of typical quality measurements applied in the study ... 76
Figure 3-6 Schematic view of heat affected zone ... 76
Figure 3-7 Optical microscopy used in this study ... 78
Figure 3-8 Scanning electron microscopy used in this study ... 79
Figure 3-9 Determination of the ferrite content in the weld seam area using the FERITSCOPE ... 79
Figure 3-10 Vickers hardness test  ... 80
Figure 3-11 Notched tensile test sample with dimension ... 81
Figure 3-12 Sequential procedure of experimental investigations ... 82
Figure 3-13 Central composite design points for three factors (i.e. f1, f2, f3) ... 83
Figure 4-1 Experimental setup used for laser welding ... 90
Figure 4-2 Effect of laser power on weld bead characteristic (focal position 0, gas pressure 1.5bar, gas flow rate 1.5lit/min) ... 93
Figure 4-3 Effect of laser power on weld width and weld area (a) Power 300W (b) Power 500W and (c) Power 800W (welding speed 15mm/s, focal position 0mm, gas pressure 1.5bar, gas flow rate 1.5lit/min) ... 94
Figure 4-4 Effect of laser power on HAZ width ... 94 Figure 4-5 Effect of laser power on HAZ width (a) power 300W (b) power 500W and (c) 800W
(welding speed 15mm/s, focal position 0mm, gas pressure 1.5bar, gas flow rate 1.5lit/min) .... 95 Figure 4-6 Effect of interaction time as a consequence of changing welding speed on weld bead characteristic ... 96 Figure 4-7 Effect of welding speed on weld width (a) 10mm/s (b) 17mm/s and (c) 35mm/s (welding power 500W, focal position 0mm, gas pressure 1.5bar, gas flow rate 1.5lit/min) ... 96 Figure 4-8 Effect of speed on HAZ width ... 97 Figure 4-9 Effect of welding speed on HAZ width (a) 5mm/s (b) 10mm/s and (c) 17mm/s (laser power 500W, focal position 0mm, gas pressure 1.5bar, gas flow rate 1.5lit/min) ... 97 Figure 4-10 Effect of specific point energy on weld beam morphology (a) 10J (b) 17J (c) 50J 98 Figure 4-11 Concept of beam position with regards to weld centreline (a) beam position toward carbon steel (b) beam position at the centre and (c) beam position toward stainless steel ... 99 Figure 4-12 Effect of beam offset on weld bead characteristic ... 100 Figure 4-13 Effect of beam positioning on weld width and weld area (a) +0.3mm toward carbon steel (b) 0mm at the centre of weld seam and (c) -0.3mm toward stainless steel (welding speed 15mm/s, laser power 500W, focal position 0mm, gas pressure 1.5bar, gas flow rate 1.5lit/min) ... 100 Figure 4-14 Effect of beam offset on HAZ width of the low carbon steel side ... 101 Figure 4-15 Effect of beam offset on HAZ width (a) +0.3mm toward mild steel (b) 0mm at the centre and (c) -0.3mm toward stainless steel (laser power 500W, laser power 500W,focal position 0mm, gas pressure 1.5bar, gas flow rate 1.5lit/min) ... 101 Figure 4-16 Variation of welding width responses in terms of laser power and welding speed (focal position 0mm, gas pressure 1.5bar, beam position at centre) ... 103 Figure 4-17 Variation of HAZ width response in terms of laser power and welding speed (focal position 0mm, gas pressure 1.5bar, beam position at centre) ... 105 Figure 4-18 Interaction effect of speed and beam position in weld bead characteristic (a) on welding width (b) on HAZ width (focal position 0mm, gas pressure 1.5bar) ... 106 Figure 5-1 Schematic diagram of a laser dissimilar welding process ... 111 Figure 5-2 Typical weld bead cross section ... 113 Figure 5-3 Typical weld bead shape and microstructure observed in dissimilar welding of low carbon to stainless steel (power = 500W, welding speed = 15mm/s) ... 115 Figure 5-4 Thermal conductivity of stainless steel and low carbon steel  ... 116
Figure 5-5 Composition of the main alloying element along the weld bead (a) Cr composition, (b) Ni composition ... 117 Figure 5-6 Effect of specific point energy on dilution (contribution of LCS to the fusion zone) ... 118 Figure 5-7 Schaeffler diagram predicting the microstructure in the fusion zone  ... 120 Figure 5-8 Microstructure of the fusion zone (a) Austenitic microstructure for specific point energy of 10J; (b) Martensitic-austenitic microstructure for specific point energy of 17J; (c) Martensitic microstructure for the specific point energy of 50J ... 121 Figure 5-9 Hardness profile versus distance from the centre of the weld ... 122 Figure 5-10 Effect of specific point energy on the weld load bearing capacity of the low carbon and stainless steel laser welded joint ... 123 Figure 5-11 Influence of specific point energy on peak load strength of the weld joint at
specific point of 17J ... 124 Figure 5-12 Beam position and alignment toward stainless steel (-) or low carbon steel (+) . 125 Figure 5-13 Effect of beam offset positions on chromium alloying concentration (inside image shows the EDS mapping of Cr element) ... 126 Figure 6-1 Mesh used for the analysis ... 130 Figure 6-2 Flowchart explaining the sequential coupling and analysis steps  ... 137 Figure 6-3 Comparison of temperature distribution for specific point energy of (a) 50J, (b) 17J, (c) 10J ... 139 Figure 6-4 Comparison of temperature inside and outside the melt pool for various specific point energies ... 140 Figure 6-5 Comparison of melting and solidification distribution profiles for specific point energy of (a) 50J, (b) 17J, (c) 10J ... 141 Figure 6-6 Comparison of top surface velocity vector for specific point energy of (a) 50J, (b) 17J, (c) 10J ... 142 Figure 6-7 Comparison of volume fraction of stainless steel for specific point energy of (a) 50J, (b) 17J, (c) 10J ... 144 Figure 6-8 Experimental hardness profile of the weld fusion zone ... 145 Figure 6-9 Comparison of experimental (left side) and simulated (right side) weld bead cross section profiles for specific point energy of (a) 50J, (b) 17J, (c) 10J ... 146
Figure 6-10 Comparison of percentage dilution of the weld bead ... 146
Figure 6-11 Von Mises stress (Pa) contour along the mid cross section profiles for specific point energy of (a) 50J, (b) 17J, (c) 10J ... 147
Figure 6-12 Von Mises stress along the middle of mid cross section of the weld sample after cool down to room temperature ... 148
Figure 7-1 Schematic of crossing: (a) High carbon steel rail, (b) High manganese steel crossing and (c) Stainless steel insert. ... 151
Figure 7-2 Schematic diagram of a laser dissimilar welding process ... 153
Figure 7-3 Optical micrograph of the parent metals and microstructures gradient in the HAZ of HCS (power = 500W, welding speed = 10mm/s, beam offset = -0.4mm) ... 157
Figure 7-4 Optical micrograph of the laser welded HCS-SS fusion zone (power = 500W, welding speed = 10mm/s, beam offset = -0.4mm) ... 158
Figure 7-5 EDX spectra and chemical analysis of ferrite region (power = 500W, welding speed = 10mm/s, beam offset = -0.4mm)... 159
Figure 7-6 Effect of alloying concentration on the microstructure (a) Primary austenitic γ dendrites (light) with interdendritic δ ferrite, (b) Martensite, (c) Martensite ... 160
Figure 7-7 Effect of cooling rate on the percentage ferrite (0.028×106°C/sec, 0.057×106°C/sec, and 0.085×106°C/sec) ... 161
Figure 7-8 Effect of cooling rate on the microstructure (a) Austenitic-martensitic microstructure, (b) Martensite, (c) Martensite ... 162
Figure 7-9 Effect of cooling rate and alloying concentration on weld microhardness ... 163
Figure 7-10 Tensile Stress-strain curve of LBW welded joint between SS and HCS ... 164
Figure 7-11 SEM micrograph of fracture surface of HCS HAZ after tensile testing ... 164
Figure 7-12 Micro-hardness profile of the dissimilar weld at various cooling rates (Cr 11%, Ni 6%) ... 165
Figure 8-1 Martensite fraction of the P92 steel pipe joint  ... 167
Figure 8-2 Post-weld heat treatment setup used for flash-butt welding ... 167
Figure 8-3 Temperature and stress history of a point in fusion zone with (Case B-2) and without (Case B-1) the consideration of martensitic phase transformation  ... 168
Figure 8-5 Martensite fraction as a function of cooling time (𝛻t8/5)for HCS ... 173
Figure 8-6 Temperature contours (K) of the HCS during the welding process ... 174 Figure 8-7 Temperature histories during laser welding for the optimum weld specimen with 25J with different distances from the fusion zone ... 174 Figure 8-8 Temperature cycle over the HCS HAZ weld for various controlled cooling time (𝛻t8/5=0.1sec, 40sec, and 140sec) ... 175
Figure 8-9 Cooling cycle between 800 to 500°C over the HCS HAZ weld for various controlled cooling time (𝛻t8/5=0.1sec, 40sec, and 140sec) ... 175
Figure 8-10 Martensite fraction (%) in HCS HAZ for various controlled cooling times (a)
𝛻t8/5=0.1sec, (b) 𝛻t8/5=40sec and (c) 𝛻t8/5=100sec ... 176
Figure 8-11 Calculated and measured martensite fraction (%) in HCS HAZ ... 177 Figure 8-12 Microhardness profile and optical micrograph of the HCS zone obtained with controlled cooling rate (𝛻t8/5=40sec) ... 177
LIST OF TABLES
Table 2-1 Typical processing parameters of CO2 laser welding ... 29
Table 2-2 Comparison of laser welding technology to other welding technologies [18, 24, 80] 40 Table 3-1 Materials used in experiments ... 70
Table 3-2 Chemical composition of the ferrous materials (wt %) ... 70
Table 3-3 Temperature dependent thermal properties of the substrate [189-192] ... 72
Table 3-4 Physical properties of the parent metals  ... 73
Table 4-1 Process parameters with design levels ... 91
Table 4-2 Central composite design experiment matrix and experimental results for this study 92 Table 4-3 ANOVA table for weld width with reduced quadratic model ... 102
Table 4-4 ANOVA table for HAZ width with reduced quadratic model ... 104
Table 5-1 Laser dissimilar welding parameters use in present investigation ... 112
Table 5-2 Average chromium and nickel equivalents calculated based on Schaeffler equivalents (gas pressure = 1.5bar, beam diameter = 0.5mm)... 119
Table 5-3 Effect of specific point energy on weld microstructure ... 120
Table 5-4 Effect of beam alignment on the composition of main alloying elements ... 125
Table 6-1 Thermal properties of the substrate ... 131
Table 7-1 Laser dissimilar welding parameters used in present investigation ... 154
Table 7-2 Effect of cooling rate and alloying concentration on weld microstructure ... 160
I would like to take this opportunity to express my deep appreciation to my supervisors Dr. Sundar Marimuthu and Prof. Jeremy Coupland for their support and encouragement. Their experience and enthusiasm were the main driving forces of this project.
I would also like to thank to all academic staff from Optical Engineering and Laser Processing Groups and Materials Engineering Department, in particular Prof. Rachel Thomson, Dr. Rebecca Higginson,Hendrik Versteeg, and Bob Temple for their kindness, friendly atmosphere and constructive discussion and advice.
Thanks to the technical staff, especially to Dave Britton, Mark Capers and Trevor Atkinson for their patience, tolerance and willingness to solve various engineering issues, as well as for being good friends.
Finally I would like to thank my wife Karbasioun (Faezeh) for taking care of me during hard times, and providing huge support, and encouragement. I would also like to thank my family for their patience and support. Special thanks should go to Dr. Keith Yendall for his mentor-like advice, and with whom much of the EDS investigation would have been mostly useless.
I hereby declare that no portion the work referred to in the thesis has been submitted in support of an application for another degree or qualification of this or any other university or other institute of learning.
LIST OF PUBLICATIONS
A list of publications taken from the thesis is given below. These are also included in full as appendices.
1. Esfahani, Reza, J. Coupland, and S. Marimuthu. "Microstructure and mechanical properties of a laser welded low carbon-stainless steel joint". Journal of Materials Processing Technology (2014).
2. Esfahani, MR Nekouie, J. Coupland, and S. Marimuthu. "Microstructural and mechanical characterisation of laser-welded high-carbon and stainless steel." The International Journal of Advanced Manufacturing Technology (2015): 1-8.
3. Esfahani, R., Marimuthu, S., and Coupland, J. “Numerical simulation and experimental investigation of laser dissimilar welding of carbon steel and austenitic stainless steel’’, ". Journal of Materials Processing Technology under publication (2015).
4. Esfahani, MR Nekouie, J. Coupland, and S. Marimuthu. "Numerical simulation and experimental investigation of laser dissimilar welding of carbon steel and austenitic stainless steel." Industrial Laser Applications Symposium 2015. International Society for Optics and Photonics, 2015.
LIST OF ACRONYMS
LDW Laser dissimilar welding
IMC Intermetallic phases or compounds YAG Yttrium – aluminium garnet
CAD Computer aided design
CAM Computer aided manufacturing CNC Computer numerical control
CW Continuous wave
EBW Electron beam welding
EDX Energy dispersive X-ray analysis SEM Scanning electron microscopy HAZ Heat affected zone
DOF Depth of focus
DoE Design of experiment
OM Optical microscopy
FW Friction welding
FSW Friction stir welding
RSM Response surface methodology BPP Beam parameter product CO2 laser Carbon dioxide laser
Introduction to Laser Dissimilar
1.1 Metal welding process
The rapid exploitation of advanced materials over the last few decades can be attributed to the developments of novel joining techniques. Welding and other joining methods are extensively used in various engineering applications, and many modern products such as cars, transportation systems, and power plants could not be possible without it. The first phase in this technological revolution occurred when welding technology replaced fastening processes. This provided enhancement in efficiency, productivity, lightweight production and surface finishing of manufactured components. Modern welding technologies, such as laser welding, friction stir welding and electro-beam welding allow joining of advanced materials. Today laser technology is revolutionising manufacturing processes due to its ease and flexibility and of non-contact processing, amenability to materials with diverse shape/geometry, properties and chemistry, and high precision/productivity.
Over the last 50 years, the availability of lasers has opened up new opportunities in industrial applications replacing many conventional welding technologies. Laser processes provide higher beam power and quality, which consequently provide higher production rate, great focusability (as a result ofdelivering precise directed energy at the desired beam shape), lower heat input and distortion, improved welding surface finish, and lower residual stress in welding. The key strength of laser beam welding (LBW) is its ability to produce a weld without defects and with a narrow heat affected zone. LBW also has the potential to produce high weld quality with control of the thermal cycle and fluid flow in the fusion zone which makes it a favourable technique for dissimilar welding of austenitic/ferritic steels. It is also worth mentioning that as a result of complex nature of the process and contribution of multiple interconnection variables, purely experimental trials cannot provide an in depth understanding of the dissimilar welding process. This requires a robust methodology for predicting the results accompanied by numerical modelling techniques  and . In general, the laser beam welding process is influenced by many parameters such as laser parameters (laser power, interaction/pulse time, gas flow rate, beam diameter, and beam alignment), thermo-mechanical properties
(thermal conductivity, coefficient of thermal expansion, etc.) and target dimensions of the workpiece (thickness, curvature, etc.).
Austenitic stainless steels and carbon steels are one of the most commonly used materials in heavy industries, especially in power generation, transportation, and petrochemical industry due their service performance, high weldability, and economical nature [3-5]. Most of the components (e.g. heat exchangers) work under different service conditions and therefore require appropriate materials. For instance components working under high temperature conditions are manufactured out of stainless steel (high oxidation resistance and creep strength) while carbon steel is used for parts working under low temperatures which make them more economical [3, 6, 7]. However there are many challenges during the welding of stainless steels to carbon steels, due to differences in thermo-physical properties and alloying composition, migration of carbon from higher carbon containing alloy to the steel with lower carbon content, residual stress, difficulties in performing post heat treatment, and metallurgical variations such as delta ferrite and sigma phases that must be carefully controlled. In addition such dissimilar joints are vulnerable to solidification cracks, uneven dilution, and phase transformation [6, 8-14]. Among these, the most critical challenges are related to martensitic phase transformation in the fusion zone and uneven dilution. The laser dissimilar welding process can be an efficient way of joining materials, however the above mentioned issues needs to be further understood.
1.2 Aims and objectives of the project
The aim of the work reported in this thesis is to investigate the basic underlying phenomena in laser dissimilar welding that influence the weld quality, through experimentation and numerical analysis. Stainless steel and carbon steel were used as the welding materials due to their wider use across range of sectors including power generation, chemical, petrochemical, and nuclear industries. Thus the following objectives were set:
• Investigate the key process variables that influence the dissimilar laser welding quality. This study will act as a foundation for further fundamental analysis.
• Investigate the significance of melt pool dynamics on microstructure, diffusion, hardness and weld strength of the dissimilar weld fusion zone.
• Develop a coupled CFD and FEM model to study the multiphase phenomena in dissimilar molten pool and to study the effect of melt pool dynamics on dissimilar weld fusion zone characteristic.
• Investigate the effect of cooling rate on the microstructure, and service performance of the dissimilar fusion zone.
• Develop a numerical model to simulate cooling rate and phase transformation in the weldment, and to study the influence of post-heat treatment on the mechanical properties of the dissimilar welded joint.
1.3 Thesis structure
This thesis presents a theoretical and experiment analysis on laser dissimilar welding of austenitic stainless steel to carbon steel. The thesis comprises of nine chapters which are described as follows.
Chapter 2 presents a fundamental review of lasers and laser welding theory. This is followed by a detailed literature review of the current state-of-the-art in welding science, including heat and mass transfer, melt pool dynamics, weld-track formation and solidification microstructure.
Chapter 3 discusses the experimental methodology and characterisation techniques used in this research. The statistical analysis technique employed with experimental results are also discussed.
Chapter 4 discusses the investigation carried out on CO2 laser dissimilar welding of low
carbon steel and stainless steel. The investigation was aimed at studying the effect of process parameters on weld quality and to establish the key process variables.
Chapter 5 investigates the effect of laser parameters on meltpool characteristics. The microstructure, diffusion, hardness and weld strength of the dissimilar weld fusion zone were studied. The influence of beam position on microstructural variations was also investigated.
Chapter 6 discusses a numerical model developed to assist in understanding the dissimilar melt pool dynamics and transportation of alloying elements. The volume of fluid technique was used to assess the dissimilar melt pool movement inside the fusion
zone. The effect of specific point energy on the weld geometry, surface morphology and mixing of the alloying elements was investigated.
Chapter 7 reports an investigation into the microstructure that arises from laser dissimilar welding of high carbon steel to austenitic stainless steel. The significance of high cooling rate and alloying composition on the microstructure and phase constitution of the dissimilar fusion zone was investigated. Typical issues that arise in welding higher carbon to stainless steel are also discussed.
Chapter 8 extends the experimental analysis described in chapter 7 and presents a sequentially coupled thermo-metallurgical finite element model, which was developed based on FLUENT code to predict cooling rate, thermal cycle and phase fraction of the heat affected zone of high carbon steel. The effect of various cooling rates on the martensitic phase transformation was also investigated. Strategies to achieve a weld that was predominantly homogenous with acceptable quality are discussed.
Chapter 9 gives a brief overview of the major conclusions and findings observed in this research as well as recommendations for future studies.
Review of the Fundamental
Theory of Laser Dissimilar Welding
Laser beam welding
This chapter presents a review of the current state-of-the-art in laser dissimilar welding (LDW). Laser fundamentals relevant to laser dissimilar welding including, lasing phenomena, laser systems and characteristics of laser beams are discussed. The basic fundamentals of laser dissimilar welding are discussed in detail and a detailed literature review on laser dissimilar welding is presented. This review includes mass and energy transfer, melt pool dynamics and weld bead formation during laser dissimilar welding. Melt pool solidification and microstructure with reference to the laser dissimilar welding were discussed. Features of laser dissimilar welding on the surface topology, geometry of the weld bead, alloying and microstructure, residual stress and distortion were also discussed.
Laser welding is a fusion welding technique used to join various materials through melting and solidification. Laser welding is predominantly used for joining components that needs high welding speeds, thin and small weld seams and low thermal distortion. According to Ribolla et al. , laser welding is one of the most robust technologies, which is widely used across various sectors including aerospace, automotive and nuclear industries.
A typical laser welding system is illustrated schematically in Figure 2-1. Laser welding process is achieved by melting the workpiece to form a weld pool/melt pool at the place of the joint followed by rapid re-solidification . The melt pool on the surface is very dynamic and is protected from oxidation typically using a shielding gas (commonly argon or helium) from the nozzle. Depending on laser power density and speed, the laser welding process can either be of keyhole or conduction welding .
Figure 2-1 Schematic illustration of laser beam welding (a) Laser welding setup (b) Close-up view of the laser welding process
2.1.1 Keyhole mode laser welding
Keyhole welding is mostly used for welding of high thickness materials  using high power density in the range of 1×106W/cm2 and 5×107W/cm2. High power density in keyhole welding leads to localized vaporization of the metals and formation of deep penetrating vapor/plasma cavity, called keyhole. The keyhole is surrounded by layers of molten materials. This layer is maintained at the equilibrium between vapor pressure (recoil pressure) and surface tension as the main driving force for keyhole formation . Hydrodynamic pressure, recoil pressure and radiation pressure helps to keep the keyhole open and make it deep while hydrostatic pressure and surface tension force help to keep the keyhole close and restricts it from becoming deeper. However, as the magnitude of the recoil pressure and surface tension pressure is significantly higher comparison to the other pressures, only these two pressures were considered during numerical calculations . Figure 2-2 illustrates the keyhole mode laser welding and cross section of laser welded sample in keyhole mode.
Figure 2-2 Keyhole laser welding (a) Schematic of keyhole mode welding and (b) Cross-section of laser welded sample in keyhole mode 
2.1.2 Conduction mode laser welding
In conduction mode, a low laser power density is applied to the weld joint, which heats up the surface of the material and melts it without any vaporization of base metals . Conduction welding is mainly used for low thickness and low penetration welding with power density less than 106 W/cm2 . The laser material interaction happens only at the surface of the work piece and the heat is transferred into the substrate by conduction and convection of molten pool. In conduction welding, the width of the weld joint on the surface is generally larger (compared to keyhole welding). The keyhole mechanism often produces welding beads with high porosity due to collapse of the keyhole and gas entrapment occurring during the solidification of the weld pool. In contrast, conduction welding is a more stable and more linear compared to keyhole welding [20-22]. It has been recently shown that the magnesium and chromium within the austenitic stainless steel weld bead is lower in keyhole mode  than conduction mode welding . Conduction welding also produces high quality smooth, rounded weld beads that do not require any extra grinding or finishing. Figure 2-3 illustrates conduction mode welding and cross section of conduction mode laser welded sample.
Figure 2-3 Conduction laser welding (a) Schematic of conduction mode welding and (b) Cross-section of laser welded sample in conduction mode 
2.1.3 Typical lasers for welding
During welding, a laser beam of sufficient intensity (or power density) is incident upon the work piece, and is moving at a constant velocity (scanning speed) to obtain a continuous weld. The laser beam intensity predominantly depends on the laser source and it significantly controls the laser welding process.
A range of laser sources, with various optical configurations were used for laser welding process. Despite recent developments in fibre laser systems, traditional lasers such as Nd:YAG and CO2 lasers are still predominantly used in industrial welding systems. CO2
lasers are reliable, robust and well-engineered industrial machines with output powers up to 50kW . The configuration of a typical CO2 laser is shown in Figure 2-4.
Figure 2-4 Configuration of a CO2 laser beam welding 
Welding with high power CO2 lasers (10.06μm wavelength) has been carried out for
well over 30 years [24-26]. Locke et al.  investigated the laser welding of stainless steel 304 with depth of penetration up to 15mm and reported that the CO2 laser welding
can be a good replacement for electron beam welding. Zhu et al.  investigated the process characteristic and mechanisms involved in diode and CO2 laser welding of
AZ31 magnesium alloy. They reported that for 1mm thick AZ31, a power density of 8000W/cm2 is desirable to obtain a full penetration at welding speed of 150mm/s employing CO2 laser or 50mm/s employing diode laser. They also reported that the spot
size of the diode laser is limited to conduction welding during defocusing, while good quality keyhole welding is produced by CO2 lasers.
The trend in laser welding applications has been toward high power CO2 welding with
continuous laser beams of 5-10kW. Modern CO2 lasers have beam qualities close to its
diffraction limit . The CO2 laser system encapsulates N2, He and CO2 gas flow in an
isolated system wherein majority of the gas is recycled via discharging process. This makes the CO2 laser operate at relatively low operational costs [18, 24].
Many researchers have recently reported the advantages of fibre lasers compared to Nd:YAG and CO2 lasers as a result of better beam quality and small beam diameter. The
higher beam quality and smaller beam diameter of fibre lasers in comparison to CO2
laser also facilitates higher penetration depth and lower residual stress/distortion . However, in contrast to their findings, there are some reports which highlight the formation of humping, porosity and pearl-like shape in the weld root due to the small diameter of the keyhole, narrow melt pool and the high surface tension involved in fibre laser welding [29-31].
Prior to the introduction of fibre laser, Nd:YAG lasers were extensively used for keyhole laser welding. Nd:YAG lasers have higher processing efficiency compared to CO2 lasers
for similar power levels. Duly  showed higher weld penetration depth with Nd:YAG welding than CO2 types for mild steel at the same power level. This is attributed to the
shorter wavelength (1.06μm) of solid state lasers (Nd:YAG), which increases the absorption level. Also the shorter wavelength enables them to be less susceptible to plasma absorption, compared to CO2 lasers. In terms of beam delivery, Nd:YAG lasers
can propagate via fibres or lens systems, whereas CO2 lasers propagate only via lens
systems. Furthermore, Nd:YAG laser provide higher pulse energies and are smaller than a CO2 lasers ,  and . However, Baardsen et al.  compared CO2 and
Nd:YAG lasers for welding of galvanized steels and showed that the CO2 laser offers
better reliability and higher welding speeds for the same power level.
Seng Ng  carried out an investigation of laser welding of high carbon steel using a pulsed 400W Nd: YAG laser, a 1.2 kW CW CO2 laser and a 1.4 kW CW high power
diode laser. He analysed and compared the weld quality of different laser systems and concluded that CO2 lasers provide a better weld quality with lower hardness profiles,
wider weld bead, higher tensile strength and greater weld volume formation.
Zhu et al.  discussed different welding mechanisms (conduction; keyhole) and studied Nd:YAG and CO2 laser welding of magnesium alloys. Hiraga et al. 
reviewed the weldability of 1.7 mm thickness wrought magnesium alloys (AZ31B-H24) using 2 kW CW CO2 and Nd:YAG lasers and concluded that the CO2 laser welded
fusion zone is lower than that produced by Nd:YAG lasers ,  and .
Baardsen et al.  performed high speed laser welding of galvanized steels using a CO2 and YAG laser. He demonstrated that the CO2 laser offers better reliability and
higher welding speeds comparison to Nd:YAG laser at similar laser power levels.
Lin Li  compared high-power diode lasers (HPDL) to Nd:YAG and CO2 lasers and
reported that a diode laser provide better surface finish, less heat-affected zone, better beam absorption as a result of its shorter wavelength and multiple beam integration during laser welding process.
Salminen et al.  made a comparison between CO2 and fibre laser to analyse the weld
penetration depth as a function of heat input (Figure 2-5) and showed that the fibre laser welding is 10–20 percent more efficient than the CO2 laser welding.
Figure 2-5 Comparison of heat input as a function of weld penetration depth for fibre and CO2 laser 
Laser welding parameters
Laser welding is controlled by many parameters including laser power, welding speed, focus position and shielding gas . In general, the weld geometry and penetration depth significantly depends on the energy per unit length which is delivered to the joint, which depends on the laser power and speed. Successful laser welding requires careful consideration of addition parameters such as the beam size, focus position, shielding gas type and flow rate and nozzle geometry. Typical parameters associated with CO2 laser
Table 2-1 Typical processing parameters of CO2 laser welding
No Parameters 1 Laser power 2 Welding speed 3 Focal position 4 Power density 5 Shielding gas
6 Welding gap and alignment 7 Wavelength
Laser beam power accompanied by welding speed is the two main important laser welding inputs which considerably influence the resulting weld. Extremely low laser power will result in a major weld defect such as lack of penetration and extremely high power will result in a drop through of the weld [41, 42].
Many researchers have highlighted the importance of laser power in welding process. Khana et al.  investigated laser welding of two different types of martensitic stainless steels (AISI 440FSe and AISI 416) employing a Nd:YAG continuous wave laser. Laser powers ranging from 800–1100 W, welding speeds ranging from 4.5–7.5 m/min and beam diameters ranging from 300-400 µm were used to study the influence of laser power, and welding speed and laser beam diameter on weld geometry and service performance. They discussed that laser power and welding speed play the most important role on shearing force and weld geometry of the weld as both affect weld resistance length and cooling rate.
Li et al.  used a continuous-wave Nd:YAG laser to weld overlap joints between H62 brass and 316L stainless steel. He investigated the influence of laser power and welding speed on microstructure, microhardness, element distribution and tensile shear strength of the dissimilar joint. They showed that above certain threshold of welding heat input (37.5 J/mm), laser power is the main factor which determines penetration-to-width ratio while below that threshold welding speed is the main parameters which affects the ratio and the weld geometry.
Kim  demonstrated that the absorptivity of the laser power is influenced by the wavelength of the laser beam and the optical properties of the workpiece material. Kim also showed that the key parameters of laser welding are the laser power, processing speed and beam diameter.
Welding speed has a significant influence on process productivity, weld pool flow pattern and fusion zone geometry. It also has inverse proportional effect on penetration depth and weld width (Figure 2-6). At low speeds the pool is large and wide, and may result in drop out. In this case the ferrostatic force is too large for the surface tension to keep the pool in place and so it drops out of the weld leaving a hole or depression. At higher speeds, the strong flow towards the center of the weld following the keyhole has no time to redistribute, and hence can solidify as an undercut at the sides of the weld . Mai and Spowage  carried out an study on pulsed Nd:YAG laser welding of dissimilar metals for three combinations of metals (steel–kovar, copper–steel and copper–aluminium). They reported a strong correlation between welding speed and weld porosity. They concluded that increasing the welding speed result in reduction of weld porosity. This is due to the fact that high speed result in shallow molten pool thus favourable condition for pores to move to the weld surface, before melt solidification.
31 Focus position
The focal plane position can have a significant effect on welding quality. Normally the focal plane is tuned to achieve maximum penetration depth and best process tolerance. El-Batahgy , investigated the relationship between the defocusing distance and penetration depth of stainless steels. His research shows that, the maximum penetration depth was observed at a defocusing distance between 0 to -1mm (Figure 2-7). However, this needs to be confirmed for each material and laser configuration. Tsukomoto et al.  showed that the depth of penetration decreases rapidly at defocus values greater than 2mm above the surface. The decrease in depth of penetration is attributed to plasma shielding. Such phenomenon is relatively trivial when the beam is focused below the surface of the workpiece.
Figure 2-7 The effect of defocusing distance on penetration depth 
Laser power density significantly influences the type of welding i.e. conduction or keyhole laser welding. Power density has a direct effect on the weld geometry and fluid flow in the fusion zone [4, 5, 18, 50, 51]. The power density at the focal point is estimated from the incident laser power and the size of the beam over the surface. For a Gaussian distributed laser beam (TEM00), the beam size is defined as the radial distance
at which the intensity of the beam decreases to 13.5% of the peak intensity . This is also the area that has approximately 87.5% of the total beam energy. The power density (intensity or irradiance),𝐼, is given by
𝐼=𝜋𝜔𝑞2 E. q(5) where 𝑞 is the power of the laser beam (W) and 𝜔 is the beam radius (mm).
0 0.25 0.5 0.75 1 1.25 1.5 1.75 2 -6 -5 -4 -3 -2 -1 0 1 2 3 4 5 P ene tr a ti o n de pt h (m m ) Defocousing distance (mm)
Torkamany et al.  carried out an investigation on dissimilar overlap welding between austhentic stainless steel and carbon steel. The influence of power density and consequent welding mode is studied on the microstructure and mechanical performance of dissimilar joint. It is showed that transition of the laser welding mode from conduction to keyhole welding as a result of power density variation have a significant impact on the dissimilar fusion zone geometry, dilution of carbon steel and consequent microstructure in the weld.
Kawahito et al.  studied the effect of laser power density on the formation of sound welds for austenitic stainless steel employing a high-power fibre laser with four different laser beams of 130, 200, 360 and 560µm spot diameters. Full penetration, without weld defects such as porosity, under filling or humping is obtained using spot diameters of 360 µm.
The relation between defects in welding with average power density, weld speed and pulse duration were investigated by Tzeng . He discussed that that the increase in weld width with increasing pulse duration is enhanced by higher average power density as a result of stronger sideways heat flow during pulsed laser welding.
Cheng et al.  investigated the Influence of power density on defect/hole and centreline cracks of stainless steel weld. They showed that that the dimension of hole formation depends on the laser power density, and the hole disappears as the power density is below 3×105 W/cm2.
Jouvard et al.  studied the Influence of power density on keyhole formation and weld depth during pulsed Nd:YAG laser welding. They reported that power density is the most critical parameter on formation of the keyhole and that the absorption of the beam increases significantly during the formation of the keyhole, and tends towards a limit value.
Mai and Spowage  performed dissimilar welding between steel–kovar, copper–steel and copper–aluminium using a pulsed Nd:YAG laser system. They reported the formation of intermetallic compound layers as undesirable compounds in the weldments. They also concluded that laser welding can minimise or avoid the formation of brittle intermetallic phases due to its locally restricted energy input and high power density.
33 Shielding gas
In laser welding the shielding gas is used to protect the weld pool from oxidation and porosity which can result in low weld quality. It also protects the beam delivery systems from metal vapor and any weld spatter. The shielding gas flow rate can also influence the melt pool stability. If it is too high, it will cool and blow away the molten metal rapidly, which result in very low welding quality. If the gas flow rate is too low, the molten pool losses its isolation from oxygen, which can oxidize the welding layer, and decrease the mechanical properties. Therefore, an optimal gas flow range should be used, that can protect both weld zone, and laser beam delivery system. It is also recommended to use Helium where high quality welds are required for materials like stainless steel, titanium, and zirconium. Argon is mostly used in the welds where oxidation is of greater concern at high temperature [18, 24].
Sattiya et al.  carried out an investigation on CO2 laser–GMAW hybrid welding with
different shielding gas mixtures (50%He + 50%Ar, 50%He + 45%Ar + 5%O2, and
45%He + 45%Ar + 10%N2) on 5 mm austenitic stainless steel sheet. It was reported that
an addition of small amount of O2 (5%) and N2 (10%) to the 50%He + 45%Ar and
45%He + 45% Ar will change the shape of the fusion zone from shallow weld to a deep and narrow fusion zone. This was attributed to the suppression of plasma plume as a result of an increases in concentration of oxygen and nitrogen .
Keskitalo et al.  studied on laser welding of duplex stainless steel using a 4 kW disk laser, with argon and nitrogen as a shielding gas. They demonstrated that use of argon as shielding gas significantly reduces the austenitic microstructure level and toughness level in weld while nitrogen as shielding gas can enhance the weld toughness. Keskitalo concluded that, nitrogen as shielding gas can compensate for loss of the elements in weld which commonly occurs during laser dissimilar welding.
Westin and Serrander  studied CO2 laser welding of duplex stainless steels and
reported that use of nitrogen as shielding gas has a positive impact on austenite formation in the root side and corrosion resistance of the weld. Similar to other researchers, it was reported that using nitrogen can prevent nitrogen loss from the weld and hence enhances austenitic formation.
34 Welding gap and alignment
Alignment of the laser beam (with reference to the weld center) and welding gap between two workpiece can significantly influence the weld bead quality. In butt joints, the gap must be small enough that the beam cannot pass straight through the joint and it was reported that the gap should be smaller than half the beam diameter (<200µm) . Sun  also demonstrated the importance of air gap size on controlling the alloying concentration of the filler wire and consequent microstructure in dissimilar laser welding between austenitic/ferritic dissimilar steel joints using nickel based filler wire. Torkamany et al. carried out an investigation on dissimilar pulsed Nd:YAG laser welding of pure niobium to Ti–6Al–4V. They discussed that laser beam alignment relative to dissimilar joint interface has significantly important role on mixing and melting ratio of fusion zone and can significantly subsidise the formation of undesirable intermetallic compounds in the weldment.
Wavelength affects the absorption, resolution and focusability. Typically, shorter wavelength has higher resolution and focusability. Shorter wavelengths have higher photon energy and higher absorption in materials for both conduction and keyhole welding. Lasers with the shorter wavelength are more desirable for keyhole laser welding where higher penetration depth is required . Figure 2-8 illustrates absorption of some metals as a function of laser radiation wavelength. Many researchers have been reported the importance of wavelength on weldability of various alloys. Sanders et al.  studied the weldability of magnesium alloys. He used Nd:YAG laser and CO2
lasers and reported that the weldability of magnesium alloys is better with Nd:YAG compared to CO2 lasers as a result of its shorter wavelength, which in turn decrease the
Figure 2-8 Absorption of a number of metals as a function of laser radiation wavelength of CO2 and YAG laser 
The effect of laser wavelength and angle of incidence on the absorptivity of wavy molten steel surfaces during welding was investigated by Kaplan . He showed that the CO2
laser has a fairly steady, high, flat-domain-absorptivity on steels molten pool from low to moderate angles-of-incidence. In addition, it is concluded that strong surface waviness of molten pool during welding enhances the absorptivity and the overall absorptance for laser wavelengths between 532 and 1070nm.
Dissimilar laser welding of metals and alloys
Dissimilar welding can be produced using various techniques, including laser beam welding, arc welding, electron beam welding, friction stir welding, etc. Tungsten inert gas (TIG) is a most well-known conventional welding technique, used for joining dissimilar materials. TIG welding uses an electric arc between a non-consumable electrode (tungsten), and workpiece to generate sufficient heat to melt the workpiece. An inert gas is used with the TIG welding to shield and cool the welding torch, welding zone, and heat affected zone . A simple configuration of the TIG welding process is shown in Figure 2-10 .
Figure 2-9 Configuration for TIG welding 
Electron beam welding is normally used to produce high quality dissimilar welding of thick materials in high value manufacturing industries. Electron beam welding is a non-conventional welding process, in which the workpiece is bombarded with a high density electrons at vacuum environment . During the electron/substrate interaction, kinetic energy of the electron converts into heat energy, which is used to melts the workpiece. Recently some non-vacuum EBW  were introduced, but still they are at the early stage of industrial implementation.
Like every process in industry, conventional arc welding has some advantages including economic, capability to weld a wide range of materials, etc. . However, large heat affected zones (HAZ) and fusion zones (FZ), high thermal residual stress and distortion, inhomogeneous microstructures and properties, evaporative loss of alloying elements and low productivity of arc-welded joints have made laser welding a preferred choice for dissimilar welding . Laser welding is preferred compared to arc welding, due to its low and precise heat input, narrow FZ and HAZ, high adaptability to automation, low residual stress and thermal distortion, and high productivity , , , ,  and . Sun and Ion  compared laser, plasma and TIG welding of austenitic/ferritic joints and showed that the width of heat affected zone in laser welded joints are approximately one-quarter and one-sixth of those in plasma and TIG welds, respectively. Sun et al.  studied dissimilar laser welded of copper and AISI 304 stainless steel and showed weld bead of superior mechanical properties compare to MIG welding.
Along with fusion welding, there are other types of joining technologies (low temperature techniques) which operate below melting temperature of base metals such as friction stir welding. Friction stir welding, developed by TWI in 1991 is a solid state welding process which produces high quality weld in difficult-to-weld materials, without melting the substrate material, and is becoming the process of choice for joining dissimilar materials . The process is achieved by using cylindrical tool which is forced on to the workpiece or parts that have already pushed together with a shoulder fixture . The tool will start to rotate and drive the separate line of the parts. As the solid tool is moving along the separation line, the heat derived by friction between the tool and the parts will soften and yield without changing the phase, (i.e. from solid to melting). The mentioned heat flow allows deformed material to relocate from the leading edge of the tool to the following edge. As a result, the material will be welded by close contact of the tool shoulder and its probe during the rotation. A schematic of the friction stir welding process is shown in Figure 2-10.
Figure 2-10 Configuration for friction stir welding 
Arivazhagan et al.  studied the microstructure and mechanical properties of stainless steel and low alloy steel using gas tungsten arc welding (GTAW), electron beam welding (EBW) and friction welding (FSW). They reported that the joint made by EBW has the highest tensile strength (681 MPa) compare to joints made by GTAW (635 MPa) and FSW (494 MPa). In addition, the ductility of the EBW and GTA weldment (32% and 25% respectively) were showed to be higher than friction weldments (19%). Impact test were also performed and it is concluded that GTAW technology produces joints with higher impact strength compare to EBW and FSW. Torkmany et al.  reported higher
service performance of dissimilar joints (carbon steel and stainless steel) welded by high energy density technologies such as laser beam welding and electron beam welding compared to conventional welding technologies.
The microstructure and mechanical properties of stainless steel welded by TIG welding, laser welding and laser-TIG hybrid welding was studied by Yan et al. . X-ray diffraction and optical microscopy are used to study the phase fraction and microstructure of the welded joint and tensile test were carried out to study the service performance of the joint. They reported that the laser welded joints had highest tensile strength and smallest dendrite size in all joints, while the TIG welded joints had lowest tensile strength, and biggest dendrite size. They also discussed higher production rate and superior mechanical properties as the advantages of laser and hybrid welding for joining austenitic stainless steel.
Sun  showed that distortion and residual stresses are significantly lower in laser welding compare to plasma and TIG dissimilar welding of austenitic stainless steel and carbon steel. He discussed that this is due to highly focused nature of the laser beam welding. Kohyama et al. [63, 72, 73] discussed that the high thickness joints made by electron beam welding have lower workpiece distortion and residual stress, higher depth to width ratio and extremely narrow heat affected zone (HAZ) compare to other welding technologies. Yunlian et al.  carried out an investigation on mechanical properties of titanium joints. They employed laser, electron beam, and TIG welding as welding technologies, and reported laser welded joints have the narrowest weld-seam, the least deformation and the finest grains among the other welding technologies as result of faster welding speed capability of laser beam welding compare to other welding technologies.
Haferkamp et al.  carried out an investigation on the fatigue performance of welded magnesium alloy components. They employed laser and electron beam as welding technologies, and reported that the laser welded joints can stand higher level of load magnitude compare to electron beam welded joints for a given number of cycles to failure. This reported to be as a result of lower notch sensitivity of laser-welded joints. Miles et al.  studied the formability of welded dual phase 590 (DP 590) steel sheets employing friction stir welding and laser welding. A series of mechanical tests, including transverse tension and plane strain formability testing are carried out. The hardness of the
weld bead was higher with laser, compared to FSW, due to the higher cooling rate with laser welding. It was also reported that FSW joints are 20% more formable than the laser welded sheets during plane strain formability tests. Sun and Duley [24, 76] discussed that friction stir welding can significantly reduce the problems associated with fusion welding due to their solid state nature; however the service conditions may make particular processes inappropriate.
The possibility of using CO2 laser-GMAW hybrid welding process was studied for the
stainless steel and influence of the shielding gas was overseen as the potent factor in the weld quality . The microstructure of the mild steel after the hybrid welding process showed coarse columnar dendrites and fine acicular dendrites in the heat affected zone (HAZ) and fine equiaxed dendrites and columnar dendrites in the weld zone. Laser zone showed the finer grain size and higher microhardness in the fusion zone and narrower heat affected zone in comparison to the arc weld region. Yan and Lee  studied the laser spot welding with the resistance spot welds (RSW) and demonstrated the weld strength of laser spot welds is greater than that of resistance spot welds. They also showed that laser spot welding can be advantageous in terms of decreasing stress distribution and welding costs in automotive industry as a result of high speed, precision and low heat distortion.
Compared to conventional arc welding, laser welding produces significantly narrower heat affected zone and fusion zone geometry (Figure 2-11). Laser welding also produces high aspect ratio welding with less distortion and residual stress in comparison with other welding methods such as conventional arc welding . Laser beam welding is predominantly carried out in ambient atmosphere (with some shielding gas), eliminating the need to control the atmospheric pressure (compare to EBW) . Also, Laser welding is fully compatible with robots to work in harsh environments (like nuclear reactors) where humans cannot operate. In addition, compared to diffusion based joining techniques such as friction stir welding, laser material processing has significantly higher productivity and flexibility for joints that have complex geometries and require non-contact welding. Despite of aforementioned advantages, laser welding is also associated with some limitations and drawbacks. Having a very high cooling rate, laser welded joints of carbon steel are often suffered from formation of martensitic phases and hot cracks in the weldments [36, 79]. Keyhole instability and formation of porosity as a result of
keyhole collapse during welding is another major drawback of laser welding. As a result of health and safety risks posed by using laser for welding this process requires researchers to undergo extensive training before they can operate it. Finally, since laser material processing is an advanced technology, it requires high amount of investments and maintenance costs compare to conventional welding technologies . Table 2-2 details the comparison of laser welding to other welding technologies.
Figure 2-11 Weld bead shape and HAZ geometry of (a) laser welded joint (power 500(W), speed 15(mm/s), argon gas pressure 1.5 (bar)) and (b) TIG welded joint (DC
current 25 Ampere, non-flow rod, thoriated tungsten electrodes)
Table 2-2 Comparison of laser welding technology to other welding technologies [18, 24, 80]
No Parameter LBW EBW TIG RW GTA GMA
1 High production rate + + +
2 Low heat input +
3 High aspect ratio + +
4 Joining efficiency +
5 Small heat affected zone + +
6 High processing speed + + +
7 Weld bead appearance + +
8 Atmospheric pressure welding + +
9 Weld reflective materials - + + + + +
10 Weld heat sensitive
materials + + - -
11 Weld magnetic materials + - + +
12 Combine with filler - + - + +
13 Automate process + - + + + 14 Operation cost - - + + + 15 Capital cost - - + + + 16 Narrow HAZ + + - 17 Environment, noise, fume + + - - 18 Fixturing + - - - - - 19 Reliability + - + + + +
'+' = advantageous; ‘-' = disadvantageous; 'LB'= laser beam; ‘EB’= electronic beam; 'RW'= resistance welding; 'GTA'= gas tungsten are 'GMA'= gas metal arc
10mm Laser welded HAZ 10mm TIG welded HAZ
As seen from the literature, welding of dissimilar metals is often involved with many challenges arising out of problems associated with metallurgical incompatibility, e.g. the formation of brittle intermetallic compounds, the segregation of high and low melting phases due to chemical mismatch, asymmetric weld pool shape, and possibly residual stresses from the thermo-physical mismatch (Figure 2-12) . Another important issue that needs to be addressed in dissimilar welding is the mutual solubility and the need for a homogenous dissimilar joint with minimal variation of mechanical properties within the weld bead and between the weld and heat affected zone. These issues are not yet fully addressed but highlighted in laser dissimilar welding research [4, 5, 24, 51, 76, 82, 83].
Figure 2-12 Welding of (a) Similar metals/alloys (b) Dissimilar metals/alloys 
Melt pool dynamics in laser welding
Melt pool convection plays a major role on final geometry, surface topology and microstructure in laser dissimilar welding. In addition, many of the weld defects such as porosity, undercuts, lack of penetration, inhomogeneous alloys and chemical composition is strongly related to the melt pool convection .
Convection in molten pool can be due to natural convection and marangoni forces. Natural convection (buoyancy) results from the change in density of the molten fluid as temperature changes. Surface tension induced convection, also known as thermocapillary flow or Marangoni flow, is caused by surface temperature gradients resulting in shear stress and induced fluid motion. The resulting flows from these forces are named as gravity-induced buoyancy convection and Marangoni convection. Marangoni driven convection forces is predominantly higher than natural convection/gravity and tend to dictate the direction of fluid flow, and the alloying composition of the fusion zone [85-87].